temperature by means of the small punch testD. Andrés 1,*, R. Lacalle 2, S. Cicero3, J.A. Álvarez4 and M. Pinzón5
1 LADICIM (Laboratory of Materials, Science and Engineering), University of Cantabria;
2 LADICIM (Laboratory of Materials, Science and Engineering), University of Cantabria;
3 LADICIM (Laboratory of Materials, Science and Engineering), University of Cantabria;
4 LADICIM (Laboratory of Materials, Science and Engineering), University of Cantabria;
4 LADICIM (Laboratory of Materials, Science and Engineering), University of Cantabria;
* Correspondence: firstname.lastname@example.org; Tel.: +34-942-200-928
Abstract: The Master Curve approach has been widely applied to characterize the ductile to brittle transition region of ferritic steels. In order to further optimise the available material to be tested, great efforts have been recently performed to combine it with miniature testing techniques. One of the most promising is the small punch testing technique, currently under standardisation process in Europe. In this paper, small punch modified specimens with a lateral notch for the estimation of fracture toughness have been employed to obtain the reference temperature, T0, of a pressure vessel steel. The influence of the applied notch length has been analysed and a valid range has been proposed. In addition, the validity criterion of the tests for the estimation of T0 has been further verified, confirming its suitability. Finally, results have been compared with those obtained with conventional fracture mechanics specimens and previous works. As a result, a methodology to estimate the reference temperature by means of small punch tests with notch lengths of approximately 4.4 mm has been proposed, turning it into a promising candidate for the characterisation of the transition regime. Keywords: small punch; reference temperature; master curve, notch, fracture toughness, transition region
The Master Curve (MC) approach enables a full characterisation of the ductile to brittle transition region of pressure vessel steels, or in general, ferritic steels, with a single parameter: the reference temperature. Developed at the VTT , the method has been successfully applied to a large number of ferritic steels and, thanks to its numerous advantages, has already been incorporated in several standards and codes, such as ASTM E1921 , BS 7910 , API 579/ASME FFS  or FKM Guideline .
One of its main features is the material optimisation: the reference temperature can be determined with a reduced number of tests. For challenging applications with reduced available material, such as the extension of the operating life of nuclear power plants, the MC approach has been combined successfully with miniature testing techniques to further reduce the material to be tested. For instance, micro compact tension specimens have been applied, employing a volume of only 10x10x4 mm per test .
The small punch technique is another promising miniature testing technique, which is currently under standardisation process in Europe . It requires reduced volumes of material to estimate its properties, with specimens of only 0.5 mm-thickness and 8mm-diameter. Thanks to its potential, it has been employed in a wide range of applications, although its origins are directly related to the assessment of the embrittlement of pressure vessel steels .
One of its most appealing applications is the estimation of fracture toughness, given the size of the specimens employed. Several approaches have been proposed, such as the use of the equivalent fracture strain  or finite element modelling , among which the use of lateral notches results highly remarkable [11, 12]. This geometry has been recently applied to the estimation of the reference temperature on several ferritic and pressure vessel steels with promising results [13, 14]. In these previous works, a fixed notch length has been employed, which might have had some influence on the results obtained. Consequently, the main goal of this paper is to analyse its effects on the estimation of the reference temperature by means of small punch specimens
with a lateral notch. To achieve it, a pressure vessel steel has been analysed and different usually employed notch-length values have been tested, in a range from 4.2 mm to 4.5 mm. In addition, the validity criterion for the tests has been confirmed, by analysing the differences in the estimations with tests exhibiting pure cleavage fractures and mixed fractures.
2. Materials and Methods
2.1. Experimental device
The small punch tests have been performed according to the recommendations of CWA 15627:2008  in a universal mechanical testing machine with a load capacity of 2.5 kN. Given the scope of the research, the testing rig has been assembled inside an environmental chamber cooled by means of liquid nitrogen, which guaranteed the attainment of the testing temperatures required to characterise the ductile to brittle transition region.
Square 10x10 mm specimens have been employed with a lateral notch on it [11, 12], as it can be seen on Figure 1, which enables the use of analytical approaches to estimate fracture toughness and that will be included in the future European Standard for small punch testing of metallic materials. Other notches have been proposed, such as the use of through thickness central notches , blind longitudinal notches  or sharp circular notches , but the lateral notch has been selected for this research given its accurate results, its ease of machining by means of wire electron cutting and the possibility of characterising any orientation of the material.
Figure 1. Scheme of a small punch specimen with a lateral notch machined on it.
To prepare the specimens, firstly the notch has been machined on 10x10 mm prisms. After this first step, it has been cut into pieces of approximately 0.55 mm thickness by means of a liquid-cooled cut-off machine. The samples have then been ground to at least 2000 grit on both sides until achieving the desired thickness of 0.5 ± 0.005 mm, according to the recommendations of CWA 15627:2008 .
The notch length has been corrected during the specimen preparation by grinding, if needed, until achieving the desired length. During the tests, the use of and adjustable lower matrix has enabled the reduction of the possible clearance between the matrix and the specimen, which could misalign the notch or vary its length. It is a novel design, which has been manufactured and validated for testing this specific geometry of specimen. It counts with a mobile piece, as shown in Figure 2, which can be adjusted to the length of each specimen, enabling the correction of the notch length if needed, something impossible to achieve by means of the conventional small punch testing rigs.
Figure 2. Adjustable lower matrix.
A pressure vessel steel, HSST A533B PLATE 13B, has been tested. Its tensile properties have been obtained by means of conventional full-scale testing techniques, as well as its reference temperature. It has a yield strength, σy, of 480 MPa, a tensile strength, σu, of 608 MPa and a reference temperature, T0, of 250 K .
2.3. Estimation of fracture toughness
The estimation of fracture toughness by means of small punch specimens with a lateral notch is based on the Crack Tip Opening Displacement (δ) concept . According to it, cracks experience a certain degree of blunting before fracture, which can be related to the toughness of the material. Shih provided evidence of a unique relationship between δ and J by evaluating the displacements at the crack tip implied by the HRR solution under elasto-plastic fracture mechanics conditions :
𝜎𝜎y , (1)
where dn is a is a dimensionless constant with a strong dependence on the strain hardening exponent of the material .
During a small punch test on a modified specimen with a lateral notch, the notch is deformed in a similar way to notch blunting, until a certain point, where a crack usually initiates. This point can be easily identified on the Force-Displacement curve as a sudden change on its slope [11, 12]. If the tests are simulated by means of finite element models, it can be seen that a material independent relationship between the degree of crack blunting or δSP and the punch displacement can be obtained for a given notch geometry, as seen in Figure 3. Consequently, δSP can be easily obtained at the point of crack initiation after the test has been performed, by simply identifying the punch displacement correspondent to the crack initiation and then by simply applying the abacus shown in Figure 3.
Figure 3. Relationship between δSP and punch displacement obtained by means of finite element models for notch lengths in between 4.2 and 4.5 mm.
If the tensile properties have already been obtained, by means of small punch tests or any other technique, equation (1) can be applied to obtain JSP. Once it has been determined, equation (2) can be employed to estimate the equivalent KJSP value at the point of crack initiation [2, 20, 22]:
𝐾𝐾J= �1−𝜈𝜈𝐸𝐸𝐽𝐽2 , (2)
where E represents the Young modulus of the material and ν is the Poisson’s coefficient.
2.4. Master Curve approach
The Master Curve approach is a statistical, theoretical, micromechanism based, analysis method for fracture toughness in the ductile to brittle transition region (DBTR) . It enables the full characterisation of the DBTR with a single material-dependent parameter, the reference temperature, which can be defined as the temperature corresponding to a KJc value of 100 MPam0.5 for a failure probability of 50%, obtained with a 25 mm-thickness specimen [1T]. 0 0,1 0,2 0,3 0,4 0,5 0,6 0,7 0,8 0,9 0 0,5 1 1,5 δSP [m m ] Punch displacement [mm] 4.2 mm 4.4 mm 4.5 mm
The MC method also takes into account the scatter of the results at the DBTR, as well as the size effects and the temperature dependence of the fracture toughness . Consequently, T0 can be obtained with a reduced number of tests with limited volumes of material by applying equation (3):
𝐾𝐾Jc [1T] = 20 + �11 + 77𝑒𝑒[0.019(𝑇𝑇−𝑇𝑇0)]� �25𝐵𝐵� 1 4�ln 1 1−𝑃𝑃f� 1 4 , (3)
where T represents the temperature in Kelvin, B is the thickness of the specimen and Pf is the probability of failure .
3. Results and discussion
3.1. Results of the small punch tests
The small punch tests have been performed at several temperatures, ranging from 143 to 158 K, for the estimation of the reference temperature. As it can be seen in Table 1, notch lengths of approximately 4.2, 4.3, 4.4 and 4.5 mm have been tested. The length values have been measured after the test, taking into account the possible deviations that the specimens might have suffered during the test, which introduce some scatter to the values. In addition, KJSP values have been estimated according to the methodology aforementioned.
Table 1. Results obtained from the small punch tests. Temperature [K] Notch length
SP [MPam0.5] Sudden force drop 158 4.19 110 158 4.19 103 153 4.22 105 × 158 4.22 103 158 4.24 84 158 4.24 110 148 4.25 82 × 148 4.27 119 153 4.29 108 153 4.29 104 153 4.29 128 153 4.30 110 158 4.38 121 148 4.39 129 143 4.40 99 × 148 4.43 105 153 4.43 133 143 4.45 122 × 148 4.46 122 153 4.46 116 148 4.49 125 153 4.51 119 × 148 4.53 98 ×
3.2. Analysis of the validity criterion
According to previous works [13, 14], to guarantee the applicability of the MC approach, the onset of cleavage cracking is the criterion of validity. After performing analysis of the micromechanisms present at the crack initiation, it has been proven that those tests exhibiting a sudden drop of the force at maximum force or those tests with a discontinuity on its slope on the proximity of maximum force exhibit pure cleavage or mixed fracture mechanisms respectively, being both valid for the determination of T0SP [13, 14].
In this paper, the effect of using the most restrictive case (sudden drop load during the test) on the reference temperature has been analysed. Consequently, the reference temperature has been estimated by applying equation (3). In one case, by only taking into account those tests with a sudden drop load and, in the other,
taking into account all of the tests, as shown in Figure 4. T0SP from pure cleavage fractures has been 146 K, while the reference temperature obtained from the whole of the tests has been 147 K.
As a result, it can be seen that the use of only pure-cleavage-fracture tests does not introduce nearly any change on the estimation of the reference temperature, being it of only 1 K in this case, in good agreement with previous analysis.
Figure 4. Small punch Master Curve obtained for all the tests performed.
3.3. Influence of the notch length on T0SP
To analyse the influence of the notch length on the estimation of the reference temperature by means of small punch tests, T0SP has been determined by applying equation (3) on groups of tests of different notch lengths, organised as following:
• 4.2 mm: tests with a notch length between 4.15 and 4.25 mm (average value: 4.22 mm). • 4.3 mm: tests with a notch length between 4.25 and 4.35 mm (average value: 4.28 mm). • 4.4 mm: tests with a notch length between 4.35 and 4.45 mm (average value: 4.41 mm). • 4.5 mm: tests with a notch length between 4.45 and 4.55 mm (average value: 4.48 mm).
The reference temperature values obtained for each notch length are shown in Figure 5. It can be clearly seen that for the shorter notches, higher small punch reference temperatures have been obtained, with a maximum difference of 20 K. On the other hand, an apparent estabilisation of the temperature seems to occur for the lengths in between 4.4 and 4.5 mm, for which practically the same T0SP value has been obtained. This effect could be due to a possible influence of the notch length on the estimations of fracture toughness for the shorter values. According to the obtained results, the use of notches shorter than 4.4 mm (for this material) leads to lower estimations of fracture toughness values, which could have risen the estimation of the reference temperature. Further research should be performed in order to achieve a better understanding of its influence.
0 50 100 150 200 250 70 120 170 220 KJc S P[M P a m 0 ,5 ] Temperature [K] KJc (0,95) KJc (0,50) KJc (0,05)
Figure 5. Small punch reference temperature obtained for each notch length.
The obtained reference temperatures for the different notch lengths have been compared with previous research [13, 14], where S275JR and S460M steels had been tested with a notch length of approximately 4.4 mm and a correlation factor between T0SP and T0 of 0.52 had been established. It can be seen that the relationship provides accurate results for all the materials tested at the same notch length, of approximately 4.4-4.5 mm. On the other hand, shorter notches lead to higher correlation values, which would increase the error of the estimation, proportional to the reduction of the notch length.
As a result, special attention should be paid to the notch length for the estimation of the reference temperature. According to the obtained results, different relationships between T0SP and T0 should be established for each specimen geometry or a single geometry should always be used. In the latter case, values in between 4.4 and 4.5 mm seem to be the most appropriate for this material, since both lengths have led to similar results.
Figure 6. Relationship between the reference temperature obtained by means of small punch tests and full-scale conventional tests for several notch lengths on A533B and for a length of 4.4 mm for S275JR and
S460M. 5. Conclusions
In this paper, the small punch testing technique has been successfully applied to the characterisation of the ductile to brittle transition region of pressure vessel steel, in combination with the Master Curve approach. Since
135 140 145 150 155 160 165 4,20 4,25 4,30 4,35 4,40 4,45 4,50 T0 S P[K ] Notch length [mm] 0 20 40 60 80 100 120 140 160 0 50 100 150 200 250 300 T0 S P[K ] T0[K] 4.22 mm 4.28 mm 4.41 mm 4.48 mm S275JR S460M 𝑇𝑇0,SP K = 0,52 𝑇𝑇0[K]
it is a model based on the direct estimation of fracture properties, small punch specimens modified with a lateral notch have been employed to estimate KJSP. It has been proven that the notch length can influence the estimated reference temperature, leading to higher values of T0SP for lengths shorter than 4.4 mm for A533B. The use of values between 4.4-4.5 mm has shown an apparent estabilisation of T0SP, with a similar correlation coefficient
T0SP-T0 to the one obtained in previous works. This could suggest that material-independent relationships between T0 and T0SP can be determined for the different notch lengths.
In addition, the test validity criterion has been further validated. It has been proven on A533B steel that both mixed fractures and pure cleavage fractures can be used to estimate T0SP without any influence on its value. Consequently, small punch tests exhibiting a discontinuity on the slope of the Force-Displacement curve or a sudden force drop can be regarded as valid. However, in case of doubt, a micromechanism analysis is encouraged to guarantee the validity of the results.
Briefly, this new approach results in a promising candidate for the characterisation of the ductile to brittle transition region of ferritic steels with an optimised use of the material. Further research is required on different materials to confirm the trends observed and achieve a better understanding of the influence of the different parameters.
Acknowledgments: This research was supported by the project MAT2014-58738-C3-3-R “Efecto del
hidrógeno en aceros de media y alta Resistencia: optimización de los métodos de caracterización para la evaluación de la integridad estructural” financed by the Ministry of Economy, Industry and Competitiveness
of the Spanish Government. References
1. Wallin, K.. Master Curve analysis of ductile to brittle transition region fracture toughness round robin data; Technical Research Centre of Finland (VTT): Espoo, Finland, 1998.
2. ASTM E1921-17a. Standard Test Method for Determination of Reference Temperature, T0, for Ferritic Steels in the
Transition Range; ASTM International: West Conshohocken, PA, 2017, DOI: 10.1520/E1921-17A.
3. BS 7910:2013+A1:2015. Guide to methods for assessing the acceptability of flaws in metallic structures; British Standards Institution: United Kingdom, 2013.
4. API 579-1/ASME FFS-1. Fitness-for-Service; American Petroleum Institute/The American Society of Mechanical Engineers, Washington, D.C., 2016.
5. FKM-Guideline. Fracture Mechanics Proof of Strength for Engineering Components, 2nd revised edition; VDMA
Publ. House: Germany, 2004.
6. Yamamoto, M.; Kimura, A.; Onizawa, K.; Yoshimoto, K.; Ogawa, T.; Chiba, A.; Hirano, T.; Sugihara, T.; Sugiyama, M.; Miura, N.; Soneda, N. A Round Robin Program of Master Curve Evaluation Using Miniature C(T) Specimens: First Round Robin Test on Uniform Specimens of Reactor Pressure Vessel Material. Proceedings of the ASME 2012 Pressure Vessels and Piping Conference, Toronto, Canada, July 15-19 2012; PVP2012-78661, 73-79, DOI: 10.1115/PVP2012-78661.
7. Bruchhausen, M.; Austin, T.; Holmström, S.; Altstadt, E.; Dymáçek, P.; Jeffs, S.; Lancaster, R.; Lacalle, R.; Matocha, K.; Petzová, J. European Standard on Small Punch Testing of Metallic Materials. Proceedings of the ASME 2017 Pressure Vessels and Piping Conference, Waikoloa, USA, July 16-20 2017; PVP2017-65396, DOI: 10.1115/PVP2017-65396.
8. Manahan, M.P.; Argon, A.S.; Harling, O.K. The development of a miniaturized disk bend test for the determination of postirradiation mechanical properties. J. Nucl. Mater 1981, 103-104, 1545-1550, DOI: 10.1016/0022-3115(82)90820-0.
9. Mao, X.; Takahashi, H. Development of a further-miniaturized specimen of 3 mm diameter for TEM disk (ϕ 3 mm) small punch tests. J. Nucl. Mater. 1987, 150:1, 45-52.
10. Abendroth, M.; Kuna, M.; Identification of Ductile Damage and Fracture Parameters from the Small Punch Test using Neural Networks. Eng. Fract. Mech. 2006, 73, 710-725, DOI: 10.1016/j.engfracmech.2005.10.007. 11. Lacalle, R.; Álvarez, J.A.; Arroyo, B.; Gutiérrez-Solana, F. Methodology for fracture toughness estimation based on
the use of Small Punch notched specimens and the CTOD concept. Proceedings of the 2nd International Conference
SSTT, Ostrava, Czech Republic, 2012.
12. Lacalle, R.; Álvarez, J.A.; Gutiérrez-Solana, F.; Use of small punch notched specimens in the determination of fracture toughness. Proceedings of the ASME 2008 Pressure Vessels and Piping Conference, Chicago, USA, July 27-31 2008; DOI: 10.1115/PVP2008-61537.
13. Lacalle, R.; Andrés, D.; Álvarez, J.A.; Gutiérrez-Solana, F. Transition Region of Nuclear Vessel Steels: Master Curve Approach Using Small Punch Notched Specimens. Key Eng. Mater. 2017, 734, 77-86, DOI: 10.4028/www.scientific.net/KEM.734.77.
14. Andrés, D.; Lacalle, R.; Cicero, S.; Álvarez, J.A.; Pinzón, M. Estimation of the reference temperature, T0, by means
of the small punch testing technique. Proceedings of the ASME 2018 Pressure Vessels and Piping Conference, Prague, Czech Republic, July 15-20 2018, PVP2018-84250.
15. Documets of CEN WS21. Small Punch Test Method for Metallic Materials, CWA 15627:2008. Part A: Code of
Practice for Small Punch Creep Testing and Part B: A Code of Practice for Small Punch Testing for Tensile and Fracture Behaviour. European Committee for Standardization, Brussels, Belgium, 2007.
16. Ju, J.B.; Jang, J.I.; Kwon, D. Evaluation of fracture toughness by small-punch testing techniques using sharp notched specimens. Int. J. PVP 2003, 80-4, 221-228.
17. Martínez-Paéda, E.; García, T.E.; Rodríguez, C. Fracture toughness characterization through notched small punch test specimens. Mater. Sci. Eng. A 2016, 657, 422-430.
18. Turba, K.; Gülcimen, B.; Li, Y.Z.; Blagoeva, D.; Hähner, P.; Hurst, R.C. Introduction of a new notched specimen geometry to determine fracture properties by small punch testing. Eng. Fract. Mech. 2011, 78-16, 2826-2833. 19. Sokolov, M.; McCabe, D.; Davidov, Y.; Nanstad, R. Use of precracked Charpy and smaller specimens to establish
the master curve. Small Specimen Test Tech. 1998, STP1329, DOI: 10.1520/STP1329-EB.
20. Anderson, T.L. Fracture Mechanics: Fundamentals and Applications, 3rd ed.; Taylor and Francis Group, 2005.
21. Shih, C.F. A Path Independent Integral and the Approximate Analysis of Strain Concentration by Notches and Cracks.
J. Appl. Mech. 1968, 35, 379-386.
22. ASTM E1820-17a. Standard Test Method for Measurement of Fracture Toughness. ASTM International: West Conshohocken, PA, 2017, DOI: 10.1520/E1820-17A.